© 2017, IRJET | Impact Factor value: 5.181 | ISO 9001:2008 Certified Journal | Page 506
“STUDY OF STRENGTH CHARACTERISTICS OF CEMENT STABILIZED
Assoc. Prof. R K Yadav2
M.E Student, Civil Engineering Department, Jabalpur Engineering college, Jabalpur (M.P)
R K Yadav: Assoc. Professor, Civil Engineering Department, Jabalpur Engineering College, Jabalpur (M.P)
Abstract:Quality aggregates are becoming increasingly scarce and expensive in many localities. In an increasing number
of cases, locally available aggregates are not meeting applicable specifications, and aggregates that meet the specifications must be imported to the site at considerable expense. The use of locally available gravel as aggregates in flexible pavement and any other field of construction is one of the best alternate for high cost of construction and a lack of quality aggregate sources .There are many methods have been tried for improving the characteristics of gravelly soil to make it suitable for intended purpose. But among various methods Stabilization of soils in order to improve strength and durability properties often relies on additives such as cement. Among various available stabilization techniques, Cement stabilization is one of the best options as it suits to any type of soil. Cement stabilized soils are widely used as construction material in sub base and base courses of pavements due to high strength and durability (Mitchell and Freitag, 1959; PCA, 1992; Ramana Murthy et al, 2006; James Isiwu Aguwa, 2009; Portelinha et al, 2012; Reddy and Prasad, 2015).
In the present work cement stabilized gravelly soil is assessing for use as an alternative concrete. Comprehensive laboratory work is carried out to study the geotechnical properties of cement stabilized gravelly soil i.e. compaction and strength characteristics of gravelly soil with cement proportions of 6%, 10%, and 14% by dry weight of the soil. The strength of cement stabilized gravel soil has been assessed after 7, 14 and 28 days of curing. Based on the results of study, the possible fields of application for use of gravel concrete are discussed. For the construction and maintenance of rural roads catering to low volumes of traffic, local soil is not only the cheapest but also the highly versatile road material.
Keywords: Cement Stabilization, Sub grade, Sub base layer, Base layer, Pavements, well graded gravel
© 2017, IRJET | Impact Factor value: 5.181 | ISO 9001:2008 Certified Journal | Page 507 advantageously used as sub-base/base for rural roads.
The soil investigated in the study is collected from gravel quarry in Gandhi gram Panagar
city, Jabalpur district in (M.P), Panagar is located at 23.3°N 79.98°E. The properties of soil determined from laboratory study are presented in Table 1. The grain size distribution curve of soil is presented in Fig.1. Based on the gradation properties, the soil is classified as well graded gravel (GW) as per BIS soil classification system. The
maximum particle size in the gravel soil collected is below 20mm size. The heavy compaction test (modified proctor test) is conducted on the soil as per IS 2720: Part 8: 1983 to evaluate compaction characteristics. The California Bearing Ratio (CBR) test is carried out as per IS 2720: part 16 (1997)  on gravel specimen compacted
under IS heavy compaction condition. The Soaked CBR value determined after soaking period
of 96 hours.
FIG. 1 0
10 20 30 40 50 60 70 80 90 100
0.01 0.1 1 10 100
% f i n e r
© 2017, IRJET | Impact Factor value: 5.181 | ISO 9001:2008 Certified Journal | Page 508 Table 1: Properties of Gravel
The cement used in the study is Birla gold 43 Grade Ordinary Portland Cement. The properties of cement determined from laboratory tests are presented in Table 2.
Specific Gravity 3.16 Initial setting time (minutes) 90 Final setting time (minutes) 418 Normal consistency (%) 30 Compressive strength (N/mm2)
i) at 3 Days 32
ii) at 7 Days 42 iii) at 28 Days 52.28
Compaction Characteristics of Cement Stabilized Gravel
The heavy compaction tests are carried out as per IS 4332 (part 3) -1995  on gravel mixed with 6, 10 and 14 percent cement content by dry weight of soil for determining compaction characteristics. Care is taken to complete the compaction test within 30 minutes from the instant of mixing of cement to soil. The OMC and MDD values of Cement stabilized GW are presented in Table 3.
S. Soil property Value
1. Grain Size Analysis
a) Gravel (%) 80
b) Sand (%) 17
c) Fines (%) 3
d) Uniformity Coefficient 5.1 e) Coefficient of Curvature 1.76 2. Plasticity Characteristics
a) Liquid limit (%) NP
b) Plastic limit (%) NP
c) Plasticity index (%) NP
3. Classification of soil GW
4. Compaction Characteristics
a) Optimum Moisture Content (%) 6.80 b) Maximum Dry Density (g/cc) 2.10
5. Soaked C.B.R (%) 30
© 2017, IRJET | Impact Factor value: 5.181 | ISO 9001:2008 Certified Journal | Page 509 It can be seen from Table 3 that the values of M.D.D values of Cement Stabilized Well graded gravel increased with increase in percentage of cement addition. However, the increment is marginal. The increased MDD values are due to filling up of voids in soil by cement. The optimum moisture content is also increased with increasing cement content under study. It is attributed to increasing the specific surface area of cement content.
Compressive strength of Cement stabilized well graded gravel is studied by varying cement content (6%, 10% and 14%). The cube specimens of size 150mmx150mmx150mm are prepared at O.M.C and respective M.D.Ds obtained from IS Heavy compaction tests. The cube specimens are cured in water for 7, 14 & 28 days and tested for the compressive strength.
The effect of addition of cement on compressive strength of cubes measured from compression tests is presented in Fig. The results depict that the strength of cement stabilized gravel increases with increase in cement percentage used for stabilization. The compressive strength of cement stabilized gravel increased with curing period.
© 2017, IRJET | Impact Factor value: 5.181 | ISO 9001:2008 Certified Journal | Page 510 It can be seen from Fig .that the compressive strength of 10 percent cement stabilized gravel cubes at 28days is 10.6 N/mm2 which is close to the strength to M10 grade conventional cement concrete. As the results of
compressive strength are encouraging, cement stabilized well graded gravel may be considered for laying bed concrete below foundations and as alternate construction material to mass concrete in gravity retaining walls construction.
Based on the results of tests conducted on cement stabilized well graded gravel under the study, the following conclusions are drawn.
1. The well graded gravel has CBR 30% and hence, it is suitable for use in its original form in sub bases of flexible pavements in rural and urban areas.
2. The gravel under study can be effectively stabilized by Cement as percentage fines is less than 5% and it is well graded.
3. The maximum dry density of cement stabilized gravel under study increased with increase in proportion of cement.
4. The compressive strength of well graded gravel increases significantly with cement stabilization.
5. The well graded gravel under study stabilized with 10 percent cement by weight may be used as alternate to lean concrete of M 10 grade.
Hence, cement stabilized well graded gravel may be used advantageously in preparation of foundation beds, sub base courses of flexible pavements and as alternate to concrete in many possible fields.
8.88 5.01 8.2 11.5 6.64 10.6 14.11 0 5 10 15 6% cement 10% cemnt 14% cement co mp re ssi ve str e n gth N /mm2
© 2017, IRJET | Impact Factor value: 5.181 | ISO 9001:2008 Certified Journal | Page 511 1. IS: 2720 Part 8 (1983): Indian Standard Code of Practice-Methods of tests for Soils-Determination of Water
Content- Dry Density Relation Using Heavy Compaction.
2. IS: 2720 part16 (1997): Indian Standard code of practice-Methods of tests for soils-laboratory determination of CBR.
3. IS: 4332 Part3 (1995): Indian Standard code of practice-Methods of tests for stabilized soils.
4. James Isiwu Aguwa (2009), “Study of Compressive Strengths of Laterite-Cement Mixes as a Building Material”, A.U.J.T, Vol.13, No.2, pp 114-120.
5. Mitchell, J.K., and Freitag, D.R (1959). “A Review and Evaluation of Soil Cement Pavements,” Journal of Soil Mechanics and Foundations Division, Proceedings of ASCE, Vol. 85, Part I, No.SM 6.
6. Portelinha F.H.M, Lima, D.C, Fontes, M.P.F and Carvalho, C.A.B (2012), “Modification of a Lateritic Soil with Lime and Cement: An Economical alternative for Flexible Pavement Layers”, Soils and Rocks, Sao Paulo, Vol.35, No.1, pp 51-63.
8. Portland Cement Association (PCA) (1992), Soil-Cement laboratory handbook, Skokie, Ill.
9. Ramanamurthy V., Deva Pratap and Hari Krishna, P (2006). “Construction and Testing of Cement Stabilized WBM Stretches”, Indian Geotechnical Conference -Chennai, India, pp 751-754.